MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS


 Ophelia Lewis
 1 years ago
 Views:
Transcription
1 MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is subjected to a compressive load and both an analytical and numerical analysis of the resulting stress fields is obtained. Some conclusions are obtained regarding the failure mode for particular examples of such cylinders. Fiber reinforced materials are being increasingly used in specialist structures where high stiffness and low weight are of considerable importance. Examples of such specialist structures are turbine blades in jet engines and racing yacht masts. Carbon fiber reinforced materials provide many of the desirable characteristics required in such applications, but they also often display some highly undesirable and sometimes unexpected properties that cause problems in their use in specialist structures. For example, although carbon reinforced turbine blades may exhibit highly desirable characteristics in the radial direction, their properties in the transverse direction may limit their usefulness in this application. Similarly, in the area of racing yacht masts, it is possible to produce a carbon reinforced cylindrical mast which has the highly desirable properties of being relatively light and also has high stiffness in the axial direction along which the fibers are aligned. Unfortunately, when subjected to standard compressive loads in the axial direction, such masts are prone to fracture and splinter as the fibers 'pop out' of the resin which binds them together to form the reinforced composite. This undesirable property needs to be suitably countered if such masts are to be useful in racing yachts. One method of overcoming the problem is to wind layers of the fiber reinforced material around the mast both on the inside and outside in order to stop the axial fibers moving out of line. These inner and outer layers do 110tsignificantly improve the strength of the material in the axial direction and of course add to the weight of the mast. It is therefore important to minimize the inner and outer layers and to include no more material than is absolutely necessary to ensure the fibers in the central layer remain in line. The purpose of the preliminary analysis in this paper is to examine the relevant stress fields with a view to determining the minimum inner and outer reinforcing layers. To this end, the stress field in a layered fiber reinforced cylinder under a compressive load is considered. Both analytical and numerical
2 solutions to the problem are obtained. Both solutions have their limitations, but nevertheless provide some insight into the important features of the problem and also provide information regarding the likely failure mode for cylinders of this type. This analysis is specific to a threelayer tubular mast structure in the form of a circular cylinder which has thin walls relative to the mast radius. The mast is fabricated from a fiberreinforced material consisting of carbon fibers set in an epoxy resin. The middle lamina is oriented with the fibres in the mast direction, and the fibres in the inner and outer layers lie at 90 to the mast axis (i.e. they are purely circumferential). The load is taken to be axial, so no moment is supported and naturally the mast is straight. The fully anisotropic behaviour of the materials is incorporated in the linear regime, so the important consequences of these properties are fully evident in the final expressions. The ratio of the stresses in all members to the applied load is obtained for all the principal directions. How these ratios vary with the design of the laminae and the elastic properties of the material is then discussed. / superscript(o,m,i) width of inner layer width of middle layer width of outer layer radius of tube Young's modulus transverse to the fibres Young's modulus in longitudinal direction (i.e. along the fibres) Poisson's ratio coupling longitudinal strain to transverse strain Poisson's ratio coupling transverse to longitudinal strain normal stress in plane 1 to mast axis (compressive taken as positive) circumferential stress (tensile taken as positive) strain in radial direction strain in longitudinal direction refers to the outer, middle or inner layers
3 The conventions for stress are not totally consistent with those used in normal engineering practice, but the final formulae are quite simple and the sense of the stress is obvious in each particular case. The final design formulae are conventionindependent. Now for a material exhibiting transverse anisotropy (i.e. rotational symmetry about the fibre axis), the stiffness matrix has only five unknowns and hence the relation va Et V/t is easy to obtain (see for example Saada, 1974). The material properties relevant to this calculation are Et El tensile strength lt l tensile strength lt t compressive strength lt l compressive strength lt t 8 GPa 125 GPa 2090 MPa 64MPa Vlt ~ MPa 210 MPa El va ~ 0.02: very little Poisson coupling in this direction. Note that, typically, (a + b + c)/r ~ 0.02, so the tube is truly thin and use of the thin walled approximation in this analysis will only cause errors of the order of 1%. Also note that Ed Et ~ 15, so the tube is much stiffer longitudinally than transversely. 4. Theory for a simple longitudinal load applied to a straight mast, prior to bending in any way. If the composite is to deform as a whole under an applied load, then the strains of each component lamina must be the same in the radial and longitudinal directions. This is the central idea in the method of consistent deformations, also called the force method (see for example Popov, 1978). Now because of the symmetry of the stress field, the tube obviously remains circular, so any strain in the circumferential direction causes an identical strain in the radial direction. Thus, for example, we can write the total radial strain of the inner layer as (i) (i) (i) ltz (To Er = va E t + E 1
4 The first term is the coupling of the strain (ui i )/ Et) caused by the normal load to the circumferential direction via Vt/, and the second term is the direct circumferential strain caused by the circumferential stress u~i)/ E/. For the other two layers, the equivalent equations are (m) (m) f(m) uz u() r V/t E/ Et (0) (0) uz f(o) u() r Vt/ E t + E/. (3) (4) Now if we consider a small section of the complete laminate, subtended by a small angle do, then there is no net radial force on such a section (such as might come from internal pressure in boiler theory). Hence the radial projection of the circumferential forces must be zero, which for unit length gives (bu~m)+ au~i) + cu~o))sin do = 0 bu~m)+ au~i) + cu~o)= o. Hence, the laminae cannot all be in either tension or compression; it will soon become clear that the stress on the middle sheet is of the opposite sign to the stress on the inner and outer strapping. Using the same idea of considering a small section subtended by the angle do and applying radial force balance, it is easy to show that the interfacial stress in the radial direction on, say, the outer lamina, is given by u(mointerface) _ c u(o) r  r (). Similar relations can be written down for the other interfaces. Most importantly, these stresses are less than the circumferential stresses by approximately a factor of 50 (c/ r, b / r, a/ r), so it is realistic to neglect the Poisson induced strains in the circumferential and longitudinal directions caused by these stresses. This is the thin shell approximation. (0) (0) (0) u() uz f/ v/t+  E/ Et (m) (m) (m) u() uz f/ Vt/ (i) Et E/ (i) u() (i) uz f/ V/t E/ + E t ' (7) (8) (9)
5 IT the laminate is not to fail between the layers, then these strains must be equal. Equating the longitudinal strains (7,8,9) then gives two independent equations, and similarly two further equations are obtained by equating the radial strains (2,3,4). The force balance (5) provides a fifth equation. Now there are six unknown stresses, O'~o),O'~m),O'~i),O'}o),O'}m) and O'}i\ so it is now possible to express all of these stresses in terms of any single one of them. It is appropriate to choose the longitudinal stress O'~m) in the middle layer as the free parameter, since it bears the bulk of the load, as will be shown shortly. Solving ( ) fi h unk (0) (m) (i) (0) (i). equations 2,3,4,5,7,8,9 or t e nowns f O'(),O'(),O'(),O'z,O'z In terms 0 O'}m) gives: 1 1 Vlt  Vtl  VltVtl Et E, (a + c)(1  vl,) b a+c b(vit  Vtl) VltVtl Et E, (a + c)(1 vl,) b. { 2 E, (a + c)(1  VltVtl) } (0) (J) 1  vit + E b E O'z 0' z t t ( ) O'(m) = O'(m) = E, (a + c)(1  vl,) El 12 z z 1 VltVtl + E t b for the longitudinal stresses. Thus, for a compressive load, all the laminae are in compression in the zdirection, and the circumferential stress is tensile in the hoop layers but compressive in the middle layer. This is intuitively very plausible. The relation (12) is most interesting. Clearly if we make the material isotropic by putting Et = E, and thus V't = Vt/, then the right hand side of (12) becomes 1, as it should, and the layers would then be indistinguishable. Alternatively, if the mast was made of three loose concentric layers (i.e. with no stress coupling between the layers), then we would expect the above ratio to be (0) (i) E O'z O'z t (m)  (m)  E,' O'z O'z as is well known. This in fact is obtainable from (12) by sending VIt, Vtl + 0 to simulate 'loose coupling'. However when the layers are glued, the tension in the outer lamina (for a compressive load) 'pulls' these layers in along the mast axis, thereby increasing the fraction of the load taken by the middle lamina rather
6 slightly. For example, with the current mast proportions of b = 2a = 2c, the factor in curly braces in (12) is about However, for any realistic values of a, band c, the curly brace factor is not going to differ appreciably from 1, so this is not a significant fact. What is interesting is that these stress ratio formulae are symmetric in a and c. More precisely they are functions only of the sum a + c. This is probably due to the thin wall approximation  the basic algebraic system that has been set up is unable to distinguish inside from outside. This may not be such an unrealistic feature as might first be supposed. It is useful to show a simplified form of the stress ratios for the special case a = c (equal thickness inner and outer hoop layers). In this case the ratios are functions of only one free parameter, a/b, and may be written in the simple forms 0.33 < a/b a/b < a/b  a/b ) ( a/b ::; with the obvious inequalities on the right. Now if we compare these expressions to the ratios tensile strength IT[ compressive strength IT[ compressive strength lt t compressive strength IT[ it is immediately clear that, for all a/b, the inner and outer layers will not fail in longitudinal tension, nor in transverse compression, before the inner lamina fails in longitudinal compression. Similarly the middle layer will not fail in transverse compression before it fails in longitudinal compression. Interestingly, these formulae indicate that even very thin hoop layers (a/b ~ 0) are at about 27% of their tensile strength, and, at worst, 52% of their transverse compressive strength, at the point where the inner layer fails in longitudinal compression.
7 A numerical analysis relevant to the problem specified in Section 2 was carried out using using the finite element package MSC/NASTRAN with bilinear quad shell elements (membrane plus bending). The analysis was based on classical bending theory. A linear static analysis was considered to examine material failure prior to buckling. Also a linear buckling analysis (eigenvalue) and a geometric nonlinear analysis (without imperfections) for local buckling of a thin shell was considered to determine the failure load due to buckling (see figures 2, 3 and 4). The results obtained are summarized in figure 1 which provides the failure load for a cylinder under compression with the total width of the cylinder wall being 1 millimeter and the percentage of the total material forming the inner and outer layers given as percentage hoop reinforcment in the graph. ~ '" 180 ~ 160 :: (> <) ~~.~ A l:: Material failure  max strain failure theory ~'local buckling  eigenvalue analysis.. l::... local buckling  geometric nonlinear analysis 100 o Figure 1: Material failure and local buckling for a carbon/epoxy Wall thickness is 1 mid. composite mast. The numerical results indicate that buckling of the mast will occur before compressive failure in the middle layer. Furthermore the results show that for a mast of 1 millimeter thickness the load at which buckling occurs is maximised by having at least 15% of the mast distributed equally in the inner and outer layers. Since it is appropriate to have as much as possible of the mast in the middle layer to support the compressive load these results suggest no more than 15% of the mast should be distributed in the inner and outer layers.
8 Local buckling is not sensitive to LID ratio
9 ...: ITr. t ~ N 10:;:.r ~ ~ I.'( ~ ~6 ~ '\ N '\:: 4I: 'J Figure 4: Linear buckling: eigenvalue analysis. (a) Compression, lowest eigenvalue. (b) Compression, higher mode. (c) Compression plus bending, lowest eigenvalue. If the possibility of buckling is ignored then the conclusion from the analysis in Sections 14 would be to make the inner and outer hoop layers as small
10 as is convenient. This is because the area of the middle lamina would need to be increased as much as possible in order to reduce the compressive stress for a given load and mast weight. This seems to be in accord with a mast constructor's observation that 'only a layer of sticky tape is needed to keep the layers in'. Accordingly, if a/ b is small, it is possible to naively obtain an upper bound for the stress in the middle lamina from equation (16), 00(m)! < IPI 1 z  21l"T(0.113a+ b)' assuming an applied compressive load P. This can be rearranged restriction to give the 0.113a + b > IPI. (20) 21l"TO'I compressive strength' but this formula is likely to grossly underestimate the required thickness since, as is clear from the numerical analysis, buckling is very likely to occur prior to pure compressive failure. Unfortunately, there are no simple analytical formulae which give a clear indication as to how the stresses vary in bending or local buckling. However, buckling formulae are usually sensitive only to elastic constants (e.g. the Euler formula or the beercan formula), so the critical buckling load of this composite is likely to be given by a complicated function of the anisotropic elastic constants only. It is difficult to estimate how this will vary with a/b. Nevertheless, the simple theory given above does give a reasonably accurate idea of how the stresses are distributed prior to failure, and thus may be of some use in the construction of yacht masts. It seems likely that, given the slenderness ratios and rigging supports used in practice, the material will fail in local buckling or longitudinal compression well before the Euler load. But consider the beercan formula for an isotropic thin cylinder of thickness h and radius T (see Timoshenko, 1961): Eh O'er = J ( 2)' T 31v If h/t ~ 1, then the buckling stress O'er is usually well below the compressive strength. Unfortunately, in the case of these masts, h/t is not especially small, so the local buckling strength is likely to be of the same order as the compressive strength. Another possible problem is that the beercan failure wavelengths might be quite large, so an experiment or finiteelement calculation might have to use a fairly long cylinder to avoid any finitelength dependence of the critical stress. The simple isotropic formulae predict about a 30 millimeter wavelength for a 92 millimeter diameter mast of thickness 1 millimeter.
11 It seems likely that a full finite element calculation has to be done to satisfactorily analyse the problem. And given the size of the 'parameter space' (the range of possible loads, afb, etc.) through which such a calculation would have to search, perhaps some restrictive decision would need to be made about the type of loads considered. The direct axial load may be a good starting point, since it can be directly compared with the preceding theory; the expressions given above are probably a good check on the finite element calculation prior to buckling. Secondly, from the simple statics of the rigging etc., it should be possible to find that part of the mast subject to the maximum moment, and use this moment plus the axial load as the load conditions in another finite element computation. Then it would be appropriate to try to maximise the load as a function of afb, as was attempted at the MISG. Naturally the finite element result would have to be meshindependent, and free of any finite length artifacts. The moderators ( David Clements and Aaron Blicblau) would like to thank Rob Denney, owner of Carbon Design, for presenting this problem. They would also like to thank James Gunning for his contribution to the analytical analysis and David Rees for his contribution to the numerical analysis. The assistance of Barrie Fraser, Vincent Hart, Walter Neumann, John Sader, Derek Wilson and Graham Wood is gratefully acknowledged. E.P. Popov, Mechanics of materials, 2nd Ed. (PrenticeHall, Englewood Cliffs, NJ,1978). A.S. Saada, Elasticity theory and applications (Pergamon Press, New York, 1974). S. Timoshenko, Theory of elastic stability, 2nd Ed. (McGrawHill, New York, 1961).
Stresses Analysis of Petroleum Pipe Finite Element under Internal Pressure
ISSN : 4896, Vol. 6, Issue 8, ( Part 4 August 06, pp.338 RESEARCH ARTICLE Stresses Analysis of Petroleum Pipe Finite Element under Internal Pressure Dr.Ragbe.M.Abdusslam Eng. Khaled.S.Bagar ABSTRACT
More informationAdvanced Structural Analysis EGF Cylinders Under Pressure
Advanced Structural Analysis EGF316 4. Cylinders Under Pressure 4.1 Introduction When a cylinder is subjected to pressure, three mutually perpendicular principal stresses will be set up within the walls
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationUnit 18 Other Issues In Buckling/Structural Instability
Unit 18 Other Issues In Buckling/Structural Instability Readings: Rivello Timoshenko Jones 14.3, 14.5, 14.6, 14.7 (read these at least, others at your leisure ) Ch. 15, Ch. 16 Theory of Elastic Stability
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationPES Institute of Technology
PES Institute of Technology Bangalore south campus, Bangalore5460100 Department of Mechanical Engineering Faculty name : Madhu M Date: 29/06/2012 SEM : 3 rd A SEC Subject : MECHANICS OF MATERIALS Subject
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationR13. II B. Tech I Semester Regular Examinations, Jan MECHANICS OF SOLIDS (Com. to ME, AME, AE, MTE) PARTA
SET  1 II B. Tech I Semester Regular Examinations, Jan  2015 MECHANICS OF SOLIDS (Com. to ME, AME, AE, MTE) Time: 3 hours Max. Marks: 70 Note: 1. Question Paper consists of two parts (PartA and PartB)
More informationMECHANICS OF MATERIALS
2009 The McGrawHill Companies, Inc. All rights reserved. Fifth SI Edition CHAPTER 3 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Torsion Lecture Notes:
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationN = Shear stress / Shear strain
UNIT  I 1. What is meant by factor of safety? [A/M15] It is the ratio between ultimate stress to the working stress. Factor of safety = Ultimate stress Permissible stress 2. Define Resilience. [A/M15]
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV UNIT I STRESS, STRAIN DEFORMATION OF SOLIDS PART A (2 MARKS)
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationQUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS
QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,
More informationCE6306 STRENGTH OF MATERIALS TWO MARK QUESTIONS WITH ANSWERS ACADEMIC YEAR
CE6306 STRENGTH OF MATERIALS TWO MARK QUESTIONS WITH ANSWERS ACADEMIC YEAR 20142015 UNIT  1 STRESS, STRAIN AND DEFORMATION OF SOLIDS PART A 1. Define tensile stress and tensile strain. The stress induced
More informationChapter 3. Load and Stress Analysis. Lecture Slides
Lecture Slides Chapter 3 Load and Stress Analysis 2015 by McGraw Hill Education. This is proprietary material solely for authorized instructor use. Not authorized for sale or distribution in any manner.
More informationLongitudinal buckling of slender pressurised tubes
Fluid Structure Interaction VII 133 Longitudinal buckling of slender pressurised tubes S. Syngellakis Wesse Institute of Technology, UK Abstract This paper is concerned with Euler buckling of long slender
More informationTorsion of shafts with circular symmetry
orsion of shafts with circular symmetry Introduction Consider a uniform bar which is subject to a torque, eg through the action of two forces F separated by distance d, hence Fd orsion is the resultant
More informationAnalysis of Composite Pressure Vessels
Analysis of Composite Pressure Vessels Reza Mohammadzadeh Gheshlaghi 1 Mohammad Hassan Hojjati Hamid Reza Mohammadi Daniali 3 1 Engineering Research Centre, Tabriz, Iran,3 Department of Mechanical Engineering,
More informationROTATING RING. Volume of small element = Rdθbt if weight density of ring = ρ weight of small element = ρrbtdθ. Figure 1 Rotating ring
ROTATIONAL STRESSES INTRODUCTION High centrifugal forces are developed in machine components rotating at a high angular speed of the order of 100 to 500 revolutions per second (rps). High centrifugal force
More informationName :. Roll No. :... Invigilator s Signature :.. CS/B.TECH (CENEW)/SEM3/CE301/ SOLID MECHANICS
Name :. Roll No. :..... Invigilator s Signature :.. 2011 SOLID MECHANICS Time Allotted : 3 Hours Full Marks : 70 The figures in the margin indicate full marks. Candidates are required to give their answers
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationME 354, MECHANICS OF MATERIALS LABORATORY COMPRESSION AND BUCKLING
ME 354, MECHANICS OF MATERIALS LABATY COMPRESSION AND BUCKLING PURPOSE 01 January 2000 / mgj The purpose of this exercise is to study the effects of end conditions, column length, and material properties
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationSTRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS
1 UNIT I STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define: Stress When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More information2012 MECHANICS OF SOLIDS
R10 SET  1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationMaterials and Shape. Part 1: Materials for efficient structure. A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka. Learning Objectives
MME445: Lecture 27 Materials and Shape Part 1: Materials for efficient structure A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Learning Objectives Knowledge & Understanding Understand the
More informationDownloaded from Downloaded from / 1
PURWANCHAL UNIVERSITY III SEMESTER FINAL EXAMINATION2002 LEVEL : B. E. (Civil) SUBJECT: BEG256CI, Strength of Material Full Marks: 80 TIME: 03:00 hrs Pass marks: 32 Candidates are required to give their
More informationEXPERIMENTAL INVESTIGATION OF INFLATABLE CYLINDRICAL CANTILEVERED BEAMS
JP Journal of Solids and Structures Volume, Issue, 2008, Pages This paper is available online at http://www.pphmj.com 2008 Pushpa Publishing House EXPERIMENTAL INVESTIGATION OF INFLATABLE CYLINDRICAL CANTILEVERED
More informationMECHANICS OF MATERIALS
GE SI CHAPTER 3 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Torsion Lecture Notes: J. Walt Oler Texas Tech University Torsional Loads on Circular Shafts
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationBISTABLE COMPOSITE SHELLS
AIAA 21385 BISTABLE COMPOSITE SHELLS K. Iqbal and S. Pellegrino Department of Engineering, University of Cambridge, Trumpington Street, Cambridge, CB2 1PZ, U.K. Abstract This paper is concerned with
More informationAccordingly, the nominal section strength [resistance] for initiation of yielding is calculated by using Equation CC3.1.
C3 Flexural Members C3.1 Bending The nominal flexural strength [moment resistance], Mn, shall be the smallest of the values calculated for the limit states of yielding, lateraltorsional buckling and distortional
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationMAHALAKSHMI ENGINEERING COLLEGE
MAHALAKSHMI ENGINEERING COLLEGE TIRUCHIRAALLI  6113. QUESTION WITH ANSWERS DEARTMENT : CIVIL SEMESTER: V SUB.CODE/ NAME: CE 5 / Strength of Materials UNIT 3 COULMNS ART  A ( marks) 1. Define columns
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More information4. BEAMS: CURVED, COMPOSITE, UNSYMMETRICAL
4. BEMS: CURVED, COMPOSITE, UNSYMMETRICL Discussions of beams in bending are usually limited to beams with at least one longitudinal plane of symmetry with the load applied in the plane of symmetry or
More informationFREE VIBRATION ANALYSIS OF THIN CYLINDRICAL SHELLS SUBJECTED TO INTERNAL PRESSURE AND FINITE ELEMENT ANALYSIS
FREE VIBRATION ANALYSIS OF THIN CYLINDRICAL SHELLS SUBJECTED TO INTERNAL PRESSURE AND FINITE ELEMENT ANALYSIS J. Kandasamy 1, M. Madhavi 2, N. Haritha 3 1 Corresponding author Department of Mechanical
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More information7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment
7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment à It is more difficult to obtain an exact solution to this problem since the presence of the shear force means that
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationCritical Load columns buckling critical load
Buckling of Columns Buckling of Columns Critical Load Some member may be subjected to compressive loadings, and if these members are long enough to cause the member to deflect laterally or sideway. To
More informationGATE SOLUTIONS E N G I N E E R I N G
GATE SOLUTIONS C I V I L E N G I N E E R I N G From (1987018) Office : F16, (Lower Basement), Katwaria Sarai, New Delhi110016 Phone : 01165064 Mobile : 81309090, 9711853908 Email: info@iesmasterpublications.com,
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationWhat to expect when you re expecting FEA A guide to good practice
What to expect when you re expecting FEA A guide to good practice 1. Background Finite Element Analysis (FEA) has transformed design procedures for engineers. Allowing more complex geometry, loading and
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationPERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK
PERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM  613 403  THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Sub : Strength of Materials Year / Sem: II / III Sub Code : MEB 310
More informationMINE ROOF SUPPORT DESIGN AND ANALYSIS. Document no : Revision no : 1.0
MINE ROOF SUPPORT DESIGN AND ANALYSIS Document no : 1806269723 Revision no : 1.0 DOCUMENT TITLE : MINE ROOF SUPPORT DESIGN AND ANALYSIS DOCUMENT NUMBER : 1806269723 ISSUE : Issue 1.0 DATE : 7 October
More informationFEA A Guide to Good Practice. What to expect when you re expecting FEA A guide to good practice
FEA A Guide to Good Practice What to expect when you re expecting FEA A guide to good practice 1. Background Finite Element Analysis (FEA) has transformed design procedures for engineers. Allowing more
More informationENG2000 Chapter 7 Beams. ENG2000: R.I. Hornsey Beam: 1
ENG2000 Chapter 7 Beams ENG2000: R.I. Hornsey Beam: 1 Overview In this chapter, we consider the stresses and moments present in loaded beams shear stress and bending moment diagrams We will also look at
More informationREPORT TO DFLEX LTD APRIL 2009 REPORT. (to DFlex Ltd, NWDA Innovation Vouchers Award, 28 April 2009)
REPORT (to DFlex Ltd, NWDA Innovation Vouchers Award, 28 April 2009) Finite Element Modelling of Rigidity of Fishing Rods with Various Crosssections Report to DFlex Ltd by Z Guan Department of Engineering,
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationCOURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5
COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5 TIME SCHEDULE MODULE TOPICS PERIODS 1 Simple stresses
More informationSimulation of Geometrical CrossSection for Practical Purposes
Simulation of Geometrical CrossSection for Practical Purposes Bhasker R.S. 1, Prasad R. K. 2, Kumar V. 3, Prasad P. 4 123 Department of Mechanical Engineering, R.D. Engineering College, Ghaziabad, UP,
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each.
GTE 2016 Q. 1 Q. 9 carry one mark each. D : SOLID MECHNICS Q.1 single degree of freedom vibrating system has mass of 5 kg, stiffness of 500 N/m and damping coefficient of 100 Ns/m. To make the system
More information: APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4021 COURSE CATEGORY : A PERIODS/ WEEK : 5 PERIODS/ SEMESTER : 75 CREDIT : 5 TIME SCHEDULE
COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4021 COURSE CATEGORY : A PERIODS/ WEEK : 5 PERIODS/ SEMESTER : 75 CREDIT : 5 TIME SCHEDULE MODULE TOPIC PERIODS 1 Simple stresses
More informationOPTIMAL DESIGN OF COMPOSITE INSERTS FOR A HYBRID ULTRACENTRIFUGE ROTOR
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS OPTIMAL DESIGN OF COMPOSITE INSERTS Hak Gu Lee 1*, Jisang Park 1, Ji Hoon Kim 1 1 Composite Materials Group, KIMS, Changwon, Korea * Corresponding
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationA STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS
Xi an, 225 th August 217 A STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS LI Zhongyang 1, LI Dong 2 Mailbox7235, Yanliang District, Xian, China, Email: zhongyangli@live.com Keywords:
More informationMAAE 2202 A. Come to the PASS workshop with your mock exam complete. During the workshop you can work with other students to review your work.
It is most beneficial to you to write this mock final exam UNDER EXAM CONDITIONS. This means: Complete the exam in 3 hours. Work on your own. Keep your textbook closed. Attempt every question. After the
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationStrength of Materials Prof S. K. Bhattacharya Department of Civil Engineering Indian Institute of Technology, Kharagpur Lecture  18 Torsion  I
Strength of Materials Prof S. K. Bhattacharya Department of Civil Engineering Indian Institute of Technology, Kharagpur Lecture  18 Torsion  I Welcome to the first lesson of Module 4 which is on Torsion
More informationMechanics of Inflatable Fabric Beams
Copyright c 2008 ICCES ICCES, vol.5, no.2, pp.9398 Mechanics of Inflatable Fabric Beams C. Wielgosz 1,J.C.Thomas 1,A.LeVan 1 Summary In this paper we present a summary of the behaviour of inflatable fabric
More informationSTRESS, STRAIN AND DEFORMATION OF SOLIDS
VELAMMAL COLLEGE OF ENGINEERING AND TECHNOLOGY, MADURAI 625009 DEPARTMENT OF CIVIL ENGINEERING CE8301 STRENGTH OF MATERIALS I 
More informationStrength Prediction Of Composite Laminate
Strength Prediction Of Composite te Prof. Yogananda. A 1, Mr. R. Vijayakumar 2 Assistant Professor, Department of Mechanical Engineering, East West Institute of Technology, Bangalore. Research Scholar,
More informationMechanical Properties
Mechanical Properties Elastic deformation Plastic deformation Fracture I. Elastic Deformation S s u s y e u e T I II III e For a typical ductile metal: I. Elastic deformation II. Stable plastic deformation
More informationEngineering Mechanics Department of Mechanical Engineering Dr. G. Saravana Kumar Indian Institute of Technology, Guwahati
Engineering Mechanics Department of Mechanical Engineering Dr. G. Saravana Kumar Indian Institute of Technology, Guwahati Module 3 Lecture 6 Internal Forces Today, we will see analysis of structures part
More informationComposite angle ply laminates and netting analysis
10.1098/rspa.2002.1066 FirstCite epublishing Composite angle ply laminates and netting analysis By J. T. Evans and A. G. Gibson School of Mechanical and Systems Engineering, University of Newcastle upon
More information18.Define the term modulus of resilience. May/June Define Principal Stress. 20. Define Hydrostatic Pressure.
CE6306 STREGNTH OF MATERIALS Question Bank UnitI STRESS, STRAIN, DEFORMATION OF SOLIDS PARTA 1. Define Poison s Ratio May/June 2009 2. What is thermal stress? May/June 2009 3. Estimate the load carried
More information8. Combined Loadings
CHAPTER OBJECTIVES qanalyze the stress developed in thinwalled pressure vessels qreview the stress analysis developed in previous chapters regarding axial load, torsion, bending and shear qdiscuss the
More informationLINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL
LINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL SREELATHA P.R * M.Tech. Student, Computer Aided Structural Engineering, M A College of Engineering, Kothamangalam 686 666,
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationCork Institute of Technology. Autumn 2007 Mechanics of Materials (Time: 3 Hours)
Cork Institute of Technology Bachelor of Engineering (Honours) in Mechanical Engineering Stage 2 (NFQ Level 8) Autumn 2007 Mechanics of Materials (Time: 3 Hours) Instructions Answer Five Questions Question
More information